Investigation of Substitution Effect on Poly(bis-3,4-ethylenedioxythiophene methine)s through Solid State Polymerization
Peng, Kai; Pei, Tong; Li, Zhaoxiang; Huang, Lili; Xia, Jiangbin; RSC Adv.  (2015) –; doi:10.1039/C5RA21122K

data_7223259
_publ_section_title
;
 Investigation of Substitution Effect on
 Poly(bis-3,4-ethylenedioxythiophene methine)s through Solid State
 Polymerization
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C5RA21122K
_journal_year                    2015
_chemical_formula_sum            'C23 H16 I2 O4 S2'
_chemical_formula_weight         674.28
_chemical_properties_physical    Heat-sensitive
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-07-06 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 106.051(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   16.947(2)
_cell_length_b                   9.1615(13)
_cell_length_c                   15.240(2)
_cell_measurement_temperature    293(2)
_cell_volume                     2273.9(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0649
_diffrn_reflns_av_sigmaI/netI    0.0731
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            21053
_diffrn_reflns_theta_full        28.35
_diffrn_reflns_theta_max         28.35
_diffrn_reflns_theta_min         2.73
_exptl_absorpt_coefficient_mu    2.978
_exptl_crystal_density_diffrn    1.970
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1296
_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent: '
_refine_diff_density_max         1.312
_refine_diff_density_min         -1.864
_refine_diff_density_rms         0.187
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.063
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     280
_refine_ls_number_reflns         5642
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.063
_refine_ls_R_factor_all          0.1349
_refine_ls_R_factor_gt           0.0735
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0895P)^2^+15.2460P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1838
_refine_ls_wR_factor_ref         0.2114
_reflns_number_gt                3338
_reflns_number_total             5642
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ra21122k2.cif
_cod_data_source_block           11
_cod_database_code               7223259